International Journal of Advanced Multidisciplinary Research
ISSN: 2393-8870 www.ijarm.com
DOI: 10.22192/ijamr Volume 4, Issue 6 -2017
Effect of different welding electrodes on welding of chrome moly steel to carbon steel material
Ramesh kumar .A1
, Senthil kumar .T2
PG student, Department of Mechanical Engineering, BIT Campus, Anna University, Trichy, Tamil Nadu, India
Dean, University College of Engineering, University, BIT Campus, Trichy, Tamil Nadu, India
The recent trend in power sector utilising alloy steels with high strength and elevated working temperature to enhance the capacity of the power plant. In view of that the boiler manufacturers concentrate on chrome molybdenum steel (gr 91).The material requires controlled process and weld procedures to maintain its mechanical and metallurgical properties. In boiler components many parts with different material specification are used.
So, the welding of dissimilar materials are inevitable. This project is to study and analyse the behaviour of chrome molybdenum steel when welded with different material specification by different electrodes using submerged arc welding process (SAW).The weld specimen subjected to different mechanical and metallurgical test.
Welding is a permanent joining process used to join different materials like metals, alloys or plastics, together at their contacting surfaces by application of heat and or pressure.
During welding, the work-pieces to be joined are melted at the interface and after solidification a permanent joint can be achieved. Sometimes a filler material is added to form a weld pool of molten material which after solidification gives a strong bond between the materials.
Weld ability of a material depends on different factors like the metallurgical changes that occur during welding, changes in hardness in weld zone due to rapid solidification, extent of oxidation due to reaction of
materials with atmospheric oxygen and tendency of crack formation in the joint position.
1.2 Different type of welding processes
Based on the heat source used welding processes can be categorized as follows:
In arc welding process an electric power supply is used to produce an arc between electrode and the work-piece material to joint, so that work-piece metals melt at the interface and welding could be done. Power supply for arc welding process could be AC or DC type. The electrode used for arc welding could be consumable or non-consumable. For non-consumable electrode an external filler material could be used.
Metal parts, Arc Welding, Grade 91 material, Carbon steel, Electrodes, Mechanical test, Metallurgical test
In gas welding process a focused high temperature flame produced by combustion of gas or gas mixture is used to melt the work pieces to be joined. An external filler material is used for proper welding. Most common type gas welding process is Oxyacetylene gaswelding where acetylene and oxygen react and producing some heat.
In resistance welding heat is generated due to passing of high amount current (1000–100,000 A) through the resistance caused by the contact between two metal surfaces. Most common types resistance welding is Spot-welding, where a pointed electrode is used.
Continuous type spot resistance welding can be used for seam-welding where a wheel-shaped electrode is used.
High Energy Beam Welding
In this type of welding a focused energy beam with high intensity such as Laser beam or electron beam is used to melt the work pieces and join them together. These types of welding mainly used for precision welding or welding of advanced material or sometimes welding of dissimilar materials, which is not possible by conventional welding process.
Solid-state welding processes do not involve melting of the work piece materials to be joined. Common types of solid-state welding are ultrasonic welding, explosion welding, electromagnetic pulse welding, friction welding, friction-stir-welding etc.
Submerged arc welding :
Submerged arc welding(SAW) involves the formation of an arc between a continuously fed electrode and the workpiece. A blanket of powdered flux which generates a protective gas shield and a slag protects the weld zone.
The arc is submerged beneath the flux blanket and is not normally visible during welding. The electrode may be a solid or cored wire or strip made from sheet. The chemical nature and size distribution of the flux assists arc stability and determines mechanical properties of the weld metal and shape of the bead. SAW is usually operated as a mechanised process. Welding current (usually 300A to 1000A),arc voltage and travel speed all
depends on parameter, position setting of filler wire.
SAW is normally operated with single wire using either AC or DC. SAW is ideally suited to the longitudinal and circumferential butt welds required for the manufacture of pipe and pressure vessels. Welding is normally carried out in flat position because of high fluidity of the weld pool and molten slag and need to maintain a flux layer.
The process has high deposition rate
Suitable for indoor and outdoor applications
No chance weld spatter Disadvantage:
Operation limited to some specific material
Operation limited to straight seam in pipe and pressure vessel
Flux handling tough
Health issue because of flux
Slag removal needed after weld Applications:
Joining of pressure vessels
Railroad construction ship building
Repairing machine parts
Many structural shapes
Scope of the project:
The main aim of the project is to study the effect of different welding electrodes on welding of chrome molybdenum steel(SA387Grade 91) to carbon steel(IS2062E240) in submerged arc welding process(SAW).
Objective of the project:
The objective of the project is to study the effect of different welding electrodes on welding of chrome molybdenum steel(SA387GR 91) to carbon steel (IS2062E240 ) using SAW (Submerged Arc Welding) process with the help of conducting and evaluating mechanical andmetallurgical tests by adopting standard codes
2.Description of test material:
2.1 Grade91 material:
It is high strength material with good creep and corrosion resistance properties.it has tempered martensitic structure with 9% chromium and
1%molybtenum and controlled addition of niobium (nb) vanadium(V) and tungsten(W).
2.2 Carbon steel:
It is high strength steel used for pressure vessel plate where the working temperature is moderate and lower.
The carbon content in this steel is 0.31 2.3 Material specification:
Table 2.3(1) Material selection for test specimen:
Description Length (MM) Width
PLATE 200 150
25 SA 387 GR 91
PLATE 200 150
Table 2.3(2) Chemical composition of the material.
Material Composition %
C Mn P S Si Cr Ni V Al Mo
SA 387GR91 0.08- 0.12
0.3-0.6 0.020 0.010 0.2-0.5 8-9.50 0.4 0.25 0.4 0.85-1.05
IS2062E240 0.23 1.50 0.045 0.045 0.40 - - - - -
Table 2.3(3) Mechanical properties of the material
Material Temperature limit
Tensile strength (MPa)
Yield strength (MPa)
SA 387 GR 91 540◦c -610◦c 585-760 415
IS2062E240 427◦c-538◦c 410 240
3.Selection of welding electrode:
Selection of welding electrode is based on the requirement of ASME boiler and pressure vessel code section-II, Part C.
An electrode is a piece of wire or a rod of a metal or alloy, with or without coatings. An arc is set up between theelectrode and work piece.
Table3.1 Chemical composition of the electrodes.
Material Composition %
C Mn P S Si Cr Ni V Cu Al Mo
0.15 1.20-1.70 0.025 0.025 0.20 - - - 0.35 - 0.45-0.65
0.15 0.40-0.80 0.25 0.25 0.05-
3.00 - - 0.35 - 0.90-1.10
0.13 1.25 0.010 0.010 0.50 8.50-
10.50 1.00 0.15-
0.25 0.10 0.10 0.85-1.15
Siddharth Pant., et al,  A good quality P91 weld joint can be obtained only when proper chemical composition of weld metal is obtained. For SMAW electrode selected for P91 steel is E-9015-B9-H4. It contains 0.08-0.13% C, 1.25 % Mn, 0.3% Si, 0.1 % S and P each, 1% Ni, 8-10.5% Cr, and 0.85-1.2% Mo.
Additional elements are V, Cu, Al, Nb, and N in small amount. The welding polarity selected is DCEP. The main thing of this electrode is that it contains very low hydrogen less than 4 ml per 100 gms of weld metal.
Backing of electrode is strongly recommended.
Though P91 material is having hardening problem during welding, it is very highly susceptible for hydrogen induced crack (HIC).
Dr. Leijun Li,  P91 material is widely used in fabrication of process equipment for nuclear and steam power plant. P91 material is having very good creep resistance and corrosion resistance at elevated temperature. This material is having low thermal coefficient of expansion. The steel ASTM A335 Gr.
P91 is a high-Cr martensitic heat-resistant steel and is applied particularly to large diameter thick-walled pipes in thermal power plants.
ZakariaBoumerzoug., et al  The study of the effect of shielded metal arc welding on industrial low carbon steel (0.19 wt. % C). The microstructures in dif-ferent zones are determined from the base metal to the weld metal. The microstructure of the center of weld zone is completely different from the heat-affected zone.
Merchant Samir Y.,  PWHT at 750°C is best suited for maintaining uniform hardness of base metal, HAZ and weld metal. It neither increases hardness of weld metal nor softness of base metal.
Talabi, S.I., et al  A significant decrease in UTS value was recorded as the current increased. The decrease in strength may be associated with the presence of void and other defects occurring as a result of increasing current. Excessive grain growth could also lead to the decrease in the tensile properties.
Asibeluo I.S., et al  The factors are responsible for the transfer mode of SMA welding. The major ones are the current, voltage, electrode diameter, melting temperature of the core material, coating thickness and
temperature of the electrode.  reported about higher penetration due to increase in Sio2 content of the flux.
It was reported that sodium and potassium salt and other elements which improved arc stability and reduced cathode spot wandering generally increased penetration.
Eroglu M ., et al  investigated the effect of coarse initial grain size with varying heat input on microstructure and mechanical properties of weld metal and heat affected zone. It was concluded that the coarse initial grain size had a great influence on the microstructure, hardness and toughness of HAZ of low carbon steel. The investigators recommended a higher heat input to obtain maximum toughness of the HAZ in the welding of grain-coarsened low carbon steel, taking into consideration the plate thickness.
From the literature survey we came to know the properties of both grade 91 steel and carbon steel. then its weldablity when welded with dissimilar materials.
The selection of welding procedures and welding electrodes. The mechanical properties of both the materials when subjected to heat and its metallurgical changes in weldment and heat affected zone, and the test procedure of the weldment to understand and analysethe changes of the weldment.
The conclusions which can be made from the review paper are study of the mechanical properties of the weld is very important because themain purpose of the welding is to strongly join thetwo metals together as the application of the welded structure may be at dynamic or static loading conditions. It is important to check the tensile strength of the weld and the factors affecting the integrity of the weld. The major problem occurs with dissimilar metal welds is susceptible to formation of inter-metallic compounds at the interface which affect the properties and efficiency of the weld.
In order to improve the strength of the dissimilar metals weld intermediate layers at the interface with suitable qualified consumables, Proper Preheat and necessary to reduce the residual stresses imparted during welding with suitable heat treatments.
7. Design of experiments:
7.1Flow diagram of experiment:
Theproposed methodology for analyzing the effect of different consumables on chrome molybtenum steel to carbon steel using shielded metal arc welding.
8.1 Experimental set up:
Experimental set up consist of welding the chrome moly plate (SA387 GR 91) with carbon steel plate (IS2062E240) by using submerged are welding(SAW) with three different welding consumablese.g EBG,EB3,EB9.
Case1: The plates are fit up with 2 mm root gap for full penetration weld. then it is preheated to 200͘◦c After reach the preheat temperature The Welding done by EBG(carbon wire)) in multiple pass bymaintaining the interpass temperature of 280˚c till the sufficient fillet is achieved by Submerged Arc Welding (SAW).After finish the weld the weld specimen subjected to post heat of 220◦c for 2 hrs.
Case2:The plates are fit up with 2 mm root gap for full penetration weld. then it is preheated to 200◦c After reach the preheat temperature The Welding done by EB3(GR 22wire) in multiple passbymaintaining the interpass temperature of 280˚c till the sufficient fillet is achieved by Submerged ArcWelding (SAW).After
finish the weld the weld specimen subjected to post heat of 220◦c for 2 hrs.
Case3:The plates are fit up with 2 mm root gap for full penetration weld. then it is preheated to 200◦c After reach the preheat temperature The Welding done by EB9(GR 91wire) in multiple passbymaintaining the interpass temperature of 280˚c till the sufficient fillet is achieved by Submerged ArcWelding (SAW).After finish the weld the weld specimen subjected to post heat of 220◦c for 2 hrs.
The welded plates are cut to suitable profiles required for the different mechanical and metallurgical tests.
The tensile and bending tests is used to measure the strength, ductility, elongation of the weld specimen.
Macro analysis of the weld is used to analyze to inspect the root fusion, metallurgy of weld,penetration of the weld etc. Soundness of weld is endured by macro analysis and optimum welding method is identified. Welding procedure and parameter for this joint developed for implementation .3D stress analysis is done using ANSYS software to ensure the new weld configuration does not generate peak stress.
8.2 Weld parameters for the process:
WIRE DIAMETE R
WELD CURRE NT
WELD VOLTA GE
RATE WELD FLUX
(EBG) 4.8mm 550A 28V 420mm/min 0.2KJ/mm TAPADIA 80
(EB3) 4.0mm 500A 28V 420mm/min 0.2KJ/mm TAPADIA 80
(EB9) 3.2mm 475A 28V 390mm/min 0.2KJ/mm MARATHAN24
8.3 Heat treatment details:
S NO HEAT TREATMENT PROCESS
RATE OH HEATING
1 STRESS RELIVING 760 ˚C 150˚C/hr 120 min
8.4 Graphical view of experimental setup
9. Mechanical tests:
9.1 Tension Tests:
The tension testing of welded joints does not specify required properties or acceptance criteria. When this standard is used as a portion of specification for a welded structure or assembly or for qualification, the following information shall be furnished:
(1) The specific type(s) and number of specimens required,
(2) Base metal specification/identification, (3) Filler material specification/identification,
(4) The anticipated property values and whether they are maximum or minimum requirements,
(5) Location and orientation of the specimens, (6) Report form when required, and
(7) Post weld thermal or mechanical processing treatments
ASME B46.1, Surface Texture, Surface Roughness, Waviness and Lay
ASTM E 4, Standard Practices for Force Verification of Testing Machines
ASTM E 8, Standard Methods for Tension Testing of Metallic Materials
ASTM B 557, Standard Test Methods for Tension Testing Wrought and Cast Aluminium and Magnesium Alloy Products
Rectangular Tension Test Specimen:
The tension specimens for welded butt joints other than pipe or tubing shall be either transverse weld tension specimens or longitudinal weld tension specimens that comply with Figure 4.2 or 4.3. When thickness of the test weldmend is beyond the capacity of the available test equipment, the weld shall be divided through its thickness into as many specimens as required to cover the full weld thickness and still maintain the specimen size within the test equipment capacity. Unless otherwise specified, the results of the partial thickness specimens shall be averaged to determine the properties of the full thickness joint.
Only ultimate tensile strength is normally determined in specimens takentransverse to the centre line of the weld.
Tensile test specimen
Universal testing machine Table 9.2Tensile test result
9.3 Bend test:
This clause covers the bend testing of fillet welds, groove welds in butt joints and the bend testing of surfacing welds. The standard gives the requirements for bend test specimen preparation, test parameters, and testing procedures, but does not specify acceptance criteria.The base materials may be homogenous, clad or otherwise surfaced, except for hard facing.
This standard is applicable to the following, where
(2) Information, specifications of acceptance, manufacturing quality control; and
(3) Research and development.When this standard is used, the following information shall be specified:(1) The specific location and orientation of the specimens;
(4) The specific types of tests, for example, face bend, side bend, or root bend and number of specimens required;
(5) Bend radius and specimen thickness (T), or percent(%) elongation. When not otherwise specified, the elongation is generally determined by the base metal or filler metal requirement, whichever is lower;
specify acceptance criteria.The base materials may be IDFN SPECIMEN SIZE IN
U.T.S in MPa POSITION OF FRACTURE
1 23.66×21.90 446 Base Metal
2 23.84×21.92 454 Base Metal
3 23.54×21.95 454 Base Metal
ASME B46.1, Surface Texture, Surface Roughness,Waviness and Lay
ASTM A 370, Standard Test Methods and Definitions for Mechanical testing of Steel Products
ASTM E 190, Standard Test Method for Guided Bend test
Bend test specimens shall be prepared by cutting the weld and the base metal to form a specimen
rectangular in cross section. For transverse bends, the surfaces cut transverse to the weld shall be designated as the sides of the specimen. For longitudinal specimens, the longitudinal surfaces that were cut to form the specimen shall be designated as the sides of the specimen and may or may not contain any weld metal. Of the two remaining fulllength surfaces, the surface with the greatest weld face width shall be designated as the face while the remaining full length surface shall be designated as the root. Transverse specimens may have the side, face, or root of the weld as the tension surface. Longitudinal specimens may have the face or the root of the weld as the tension.
9.5 Table Bend test result:
IDENTIFICATION SIDE BEND REMARKS
11 No open discontinuity passed
12 No open discontinuity passed
21 No open discontinuity passed
31 No open discontinuity passed
32 No open discontinuity passed
Bend test specimen 9.6 Impact test:
Impact test is carried out to measure and identify the behaviour of each material when subjected to sudden load.
9.7 Table Impact test result:
IDFN IMPACT ENERGY IN
JOULES IDFN IMPACT ENERGY IN
11 119 23 87
12 113 24 82
13 103 31 16
14 114 32 18
21 78 33 23
22 89 34 16
Impact test specimen 10.1Microhardness measurements:
Micro indention hardness measurement is performed
the Basemetal, heat affected zone and buffer layers at a load of 200g in the interval 2000 micron distance by usingmicro indention hardness tester(Vickers
10.2 Table Vickers hardness in vertical:
METAL HAZ BASEMETAL
EBG 1 153 166 197 200 211
EBG 2 157 165 212 222 192
EBG 3 183 190 280
EBG 4 162 187 234
EB3 1 175 210 192 218 213
EB3 2 175 202 199 210 243
EB3 3 190 200 217
EB3 4 196 213 222
EB9 1 175 313 239 305 300
EB9 2 186 267 273 296 257
EB9 3 158 270 233
EB9 4 178 308 233
10.3 Macro& microstructure:
Micro test is conducted by optical microscope at differentfocal length to find out the microstructure present in theweld metal, HAZ, weld interface, Root interface and basemetal.Metallography procedure is used to study the microstructureof base metals, weld
metals and heat affected zone andmicrostructure changesThe recording observed under metallurgical microscope canbe the effective way to analysis the effectsOf cladding layers base plate and SA387 GR91&IS2062.Microstructure reveals the better bonding of SA387 GR 91 isobserved with lesser dilution as compared to IS2062.
Macroimage of sample1 Macro image of sample2
Macro image of sample 3
Fig 1MicrostructureofmetalIS2062-100Xfig 2Microstructure of metal SA387 GR 91-200X
Fig5 Microstructure of weldment (EBG)-200X fig6 Microstructure of weldment(EBG)-500X
Fig7Microstructure of metal IS2062-100X fig8 Microstructure of metal SA387 GR91-100X
Fig9 MicrostructureofHAZIS2062-100X fig10Microstructureof HAZSA387GR91-100X
Fig11 Microstructure of weldment (EB3)-100X fig12 Microstructure of weldment(EB3)-200X
Fig13 Microstructure of metalIS2062-100X fig14 Microstructure of metal SA387GR91-200X
Fig17 Microstructure of weldment (EB9)-200X Fig18 Microstructure of weldment(EB9)-500X
The conclusions which can be made from the review papers are study of the mechanical properties of the weld is very important because the main purpose of the welding is to strongly join the two metals together as the application of the welded structure may be at dynamic or static loading conditions. It is important to check the mechanical properties and metallurgical changes occurred duo to welding of dissimilar materials and the various factors affecting the weldment dueto specific property of each material.
The experiment performed based on standard codes and procedures. The various test report reveals that the property of the two test materials(SA387GR91 and IS2062E240) doesn’t change too much while welding together.From the tensile test the probability of weld failure occurs at low grade material at given load, from impact test we can understand the failure occurs at high chrome materials and micro and macro analysis indicates soundness of the weld and metallurgical changes of the material. This thesis of report concludes that the welding of these two dissimilar material using different electrodes can provide a quality weld in terms of mechanical and metallurgical aspects. but, the selection of welding electrode and process should be selected based on its working condition and type of load might encounter the weld joint.
 Siddharth Pant and Swati Bhardwaj, “Properties and Welding Procedure for Grade 91 Alloy Steel”, International Journal of Engineering Research and
Technology, Volume 6, Number 6 (2013), pp. 767- 772.
 Dr. Leijun Li, “Effect of Post-Weld Heat Treatment on Creep Rupture Properties of Grade 91 Steel Heavy Section Welds”, Mechanical & Aerospace Engineering, Utah State University (435)797-8184, 2012.
 Zakaria Boumerzoug1, Chemseddine Derfouf1, Thierry Baudin Effect of Welding on Microstructure and Mechanical Properties of an Industrial Low Carbon Steel,http://www.SciRP.org/journal/engJuly 2010.
integrity of the weld. The major problem occurs with dissimilar metal welds is susceptible to formation of inter-metallic compounds at the interface which affect the properties and efficiency of the weld. In order to improve the strength of the dissimilar metals weld intermediate layers at the interface with suitable qualified consumables, Proper Preheat and necessary to reduce the residual stresses imparted during welding with suitable heat treatments.
 Merchant Samir Y A Review Of Effect Of Welding And Post Weld Heat Treatment On Microstructure And Mechanical Properties Of Grade 91 Steel
International Journal of Engineering Research and Technology, Mar-2015 Volume 04 Issue 03.
 Talabi, S.I.a,*, Owolabi, O.B.b, Adebisi, J.A.a, Yahaya, T Effect of welding variables on mechanical properties of low carbon steel welded joint Advances in Production Engineering & Management Volume 9, Number 4, December 2014, pp 181–186.
 Asibeluo I.S, Emifoniye E. Effect of Arc Welding Current on the Mechanical Properties of A36 Carbon Steel Weld JointsSSRG International Journal of Mechanical Engineering (SSRG-IJME) – volume 2 Issue 9 – September 2015
Access this Article in Online Website:
Quick Response Code
How to cite this article:
Ramesh kumar .A , Senthil kumar .T. (2017). Effect of different welding electrodes on welding of chrome moly steel to carbon steel material. Int. J. Adv. Multidiscip. Res. 4(6): 64-79.